Coprecipitated ferrite nanoparticles were coated with carbon using a hydrothermal method. From transmission electron microscope pictures, we could see that the coated iron oxide nanoparticles were spherical in shape with an average diameter of 90 nm. The strong bonding of carbon on the nanoparticle surfaces was checked by noting the C = O and C = C vibrations in Fourier transform infrared spectra. The spin-lattice relaxation process [T1] and spin-spin relaxation process [T2] relaxivities of hydrogen protons in the aqueous solution of coated nanoparticles were determined to be 1.139 (mM·s)-1 and 1.115 (mM·s)-1, respectively. These results showed that the carbon-coated iron oxide nanoparticles are applicable as both T1 and T2 contrast agents in magnetic resonance imaging.
PACS: 81.05.y; 76.60.Es; 61.46; 75.50.k; 87.61.
Nanostructured materials have attracted a great deal of attention in the development of biotechnology and medicine [1–3]. Among these nanostructured materials, carbon-coated metal oxide nanoparticles such as MgO, CaO, ZnO, TiO2, Al2O3, and Fe2O3 are now extensively studied because of their high application potential [4–9]. Recently, much research interest has been expended on the ferromagnetic iron oxide materials generally used for magnetic data storage as magnetic toners in xerography, and on the ferrofluids, used as contrast agents in magnetic resonance imaging [MRI] [10–13].
The carbon coating provides an effective oxidation barrier and prevents corrosion in magnetic core materials. Hydrophilic carbon coating on iron oxide nanoparticle cores endows better dispersibility and stability than those shown by bare iron oxide nanoparticles. In general, different approaches have been employed for the synthesis of carbon coatings, for example, electric arc discharge, catalytic pyrolysis of organic compounds, and the hydrothermal methods .
In this paper, we report the synthesis of carbon coating on iron oxide (Fe3O4) nanoparticles by a hydrothermal method proposed by Zhang et al.  with some modifications. We evaluated these coated particles as potential spin-lattice relaxation process [T1] and spin-spin relaxation process [T2] contrast agent in MRI. We studied the T1 and T2 relaxations of hydrogen protons in water molecules in an aqueous solution of carbon-coated iron oxide nanoparticles. We found that the T1 and T2 relaxivities for the aqueous solution of carbon-coated iron oxide nanoparticles were 1.139 and 1.115 (mM·s)-1, respectively. The ratio of these two relaxivities is close to unity. This result demonstrates that carbon-coated iron oxide nanoparticles are suitable as both T1 and T2 contrast agents in MRI.
Materials and fabrication
Carbon-coated iron oxide nanoparticles were synthesized by hydrothermal synthetic processes. Bare iron oxide nanoparticles were formed using the coprecipitation method, in which NaOH solution was slowly added to a mixed solution of ferric and ferrous chlorides in a glove box filled with argon gas. During this process, iron oxide nanoparticles were precipitated. These magnetic particles were separated by a magnet and were washed out by methanol, acetone, and DI [deionized] water. The collected nanoparticles were dried in a vacuum oven to obtain a powder sample of nanoparticles for coating. The dried nanoparticles were dispersed in a solution of 0.5 M glucose for 5 h with sonification. During this process, carbon was coated onto the surfaces of the nanoparticles. The solution was dried in a vacuum oven filled with argon gas for 4 h. The dried, coated nanoparticles were redispersed in DI water and filtered through a 100-nm filter paper several times.
The particle size distribution and structure of the carbon-coated nanoparticles were checked using a TEM microscope (TEM, H-7600, Hitachi High-Tech, Minato-ku, Tokyo, Japan). The hydrodynamic diameter and diffusion constant of the coated nanoparticles in water were measured with a dynamic light scattering [DLS] particle size analyzer (ELSZ-2, Otsuka Electronics Co., Ltd., Osaka, Japan). The bonding of carbon onto the iron oxide particles were confirmed by using Fourier transform infrared spectroscopy [FTIR]. For the relaxivity measurements, aqueous solutions of various nanoparticle concentrations were prepared. The concentration of nanoparticles in the aqueous solution was measured with an inductively coupled plasma [ICP] spectrophotometer (IRISAP, Thermo Jarrell Ash, Franklin, MA, USA). The T1 and T2 relaxation times of hydrogen protons in the aqueous solution of the coated nanoparticles were measured using an MR scanner (1.5 T Scanner, GE Medical System, Saskatchewan, Canada).
Results and discussion
Figure 1 shows TEM images for the carbon-coated iron oxide nanoparticles. The TEM images showed that the coated nanoparticles were spherical in shape with an average diameter of 90 nm. The average hydrodynamic diameter of the carbon-coated nanoparticles measured by a DLS particle size analyzer was about 200 nm (Figure 2). This diameter was larger than the value measured by TEM due to both surface coating of the nanoparticles and the water solvation around the nanoparticles. The diffusion constant of the nanoparticles in water was 9.7265 × 10-9 cm2/s.
The bonding status of carbon on the surfaces of the nanoparticles was checked using the wavelength-dependent transmittance data obtained using an FTIR spectrometer (Nicolet 380, Thermo Scientific, Waltham, MA, USA). Figure 3a, b shows the FTIR spectra for bare iron oxide and carbon-coated iron oxide nanoparticles, respectively. The bands at 1,700 and 1,610 cm-1 in the spectra of carbon-coated iron oxide are associated with the C = O and C = C vibrations, respectively, which resulted from the carbonization of glucose during the hydrothermal reaction [14, 15]. The peaks at 1,000 to approximately 1,400 cm-1 are attributed to the C-OH stretching and O-H bending vibrations. The band at 2,920 cm-1 resulted from the stretching vibrations of O-H.
To demonstrate the T1 and T2 effects in an aqueous solution, MR images for aqueous solutions of various nanoparticle concentrations were obtained. We prepared ten different samples with varying concentrations (ranging from 0.427 to 4.27 mM of iron) of nanoparticles in DI water and put them into microfuge tubes for imaging. One example of the MR images is shown in Figure 4.
In MRI, the signal recorded during the scan is related to the magnetic relaxation processes of the nuclear spins of the protons in the water molecules in the area of interest. Under a given external magnetic field (B), the nuclear spins of the protons align with the field, giving rise to a net magnetization, M. If a radio frequency [rf] pulse is perpendicularly applied to B, the nuclear spins are excited and start precessing in the plane perpendicular to B. Upon removal of the rf pulse, the nuclear spins gradually recover to their equilibrium state parallel to B. The recovery of the equilibrium takes place via two different relaxation mechanisms: the spin-lattice relaxation process (T1), or in other words, the recovery of the magnetization along the B direction, and the spin-spin relaxation process (T2), i.e., the loss of signal in the perpendicular plane. The presence of nanoparticles in the area of interest creates an additional magnetic field (B1) which induces local field inhomogeneities that significantly increase the speed of the proton transverse relaxation (decrease of T2), leading to a negative contrast or a darkening of the image.
For T1 measurements, the inversion recovery pulse sequence was used. In this pulse sequence, the relaxation of nuclear spins in the aqueous solution of the magnetic nanoparticles can be expressed in the following equation:
The signal intensities for 35 different times of inversion ranging from 50 to 1,750 ms can be obtained from these MR images. By applying these data to the intensity function of the MR signal, we can obtain the T1 relaxation time. Figure 5 shows the plot for two different samples of nanoparticles with concentrations of 0.427 and 4.27 mM iron.
The Carr-Purcell-Meiboon-Gill pulse sequence with multiple spin echo was used for the T2 measurements. MR images for 30 different times of echo ranging from 10 to 1,700 ms were obtained. For the signal intensity function of T2 relaxation, the following relationship was used to determine the T2 relaxation times:
Figure 6 shows the plot for two different samples of nanoparticles with concentrations of 0.427 and 4.27 mM iron. The relaxivities of nuclear spins in an aqueous solution of magnetic nanoparticles can be expressed as :
where i = 1 or 2, and represents the relaxivity of nuclear spins with no nanoparticle contrast agent. Also, R i is the relaxivity of nuclear spins per mM of nanoparticles, and C represents the concentration of nanoparticles in the aqueous solution.
Figure 7 represents the plots of and as a function of the concentration of carbon-coated nanoparticles. The slopes of the straight lines are 1.139 and 1.115 (mM·s)-1, respectively. The ratio of these two relaxivities was close to unity. This result demonstrates that carbon-coated iron oxide nanoparticles are suitable as both T1 and T2 agents for MRI.
We synthesized highly water-dispersible carbon-coated iron oxide nanoparticles for use as contrast agents in MRI. The coated nanoparticles were observed to be spherical with a core-shell structure in the TEM images, and they showed a uniform size distribution with an average diameter of 90 nm. The strong bonding of carbon on the nanoparticle surfaces was checked by noting the C = O and C = C vibrations in FTIR spectra. The T1 and T2 relaxation times of hydrogen protons were measured using an MRI scanner in the aqueous solutions of various concentrations of nanoparticles ranging from 0.427 to 4.27 mM. The T1 and T2 relaxivities were 1.139 and 1.115 (mM·s)-1, respectively. The ratio of these two relaxivities was close to unity. This result shows that carbon-coated iron oxide nanoparticles are suitable as both T1 and T2 contrast agents in MRI.
dynamic light scattering
Fourier transform infrared
inductively coupled plasma
magnetic resonance imaging
transmission electron microscope.
Huang SH, Liao MH, Chen DH: Direct binding and characterization of lipase onto magnetic nanoparticles. Biotechnol Prog 2003, 19: 1095–1100. 10.1021/bp025587v
Josephson L, Perez JM, Weissleder R: Magnetic nanosensors for the detection of oligonucleotide sequences. Angew Chem Int Ed 2001, 40: 3204–3206. 10.1002/1521-3773(20010903)40:17<3204::AID-ANIE3204>3.0.CO;2-H
Katz E, Sheeney-Haj-Ichia L, Buckmann AF, Willner I: Dual biosensing by magneto controlled bioelectrocatalysis. Angew Chem Int Ed 2002, 41: 1343–1346. 10.1002/1521-3773(20020415)41:8<1343::AID-ANIE1343>3.0.CO;2-K
Khaleel A, Kapoor PN, Klabunde KJ: Nanocrystalline metal oxides as new adsorbents for air purification. Nanostruct Mater 1999, 11: 459–468. 10.1016/S0965-9773(99)00329-3
Koper OB, Lagadic I, Volodin A, Klabunde KJ: Alkaline-earth oxide nanoparticles obtained by aerogel methods. Characterization and rational for unexpectedly high surface chemical reactivities. Chem Mater 1997, 9: 2468–2480. 10.1021/cm970357a
Klabunde KJ, Stark JV, Koper OB, Mohs C, Park DG, Decker Jiang SY, Lagadic I, Zhang D: Nanocrystals as stoichiometric reagents with unique surface chemistry. J Phys Chem 1996, 100: 12142–12153. 10.1021/jp960224x
Wagner GW, Koper OB, Lucas E, Decker S, Klabunde KJ: Reactions of VX, GD, and HD with nanosize CaO: autocatalytic dehydrohalogenation of HD. J Phys Chem B 2000, 104: 5118–5123. 10.1021/jp000101j
Jang HD, Kim SK, Kim SJ: Effect of particle size and phase composition of titanium dioxide nanoparticles on the photocatalytic properties. J Nanopart Res 2001, 3: 141–147. 10.1023/A:1017948330363
Miller TM, Grassian VH: Adsorption and decomposition of nitrous oxide on zirconia nanoparticles [abstract]. Colloids Surf A 1995, 105: 113. 10.1016/0927-7757(95)03299-7
Kim J, Lee JE, Lee SH, Yu JH, Lee JH, Park TG, Hyeon T: Designed fabrication of a multifunctional polymer nanomedical platform for simultaneous cancer-targeted imaging and magnetically guided drug delivery. Adv Mater 2008, 20: 478–483. 10.1002/adma.200701726
Senpan A, Caruthers SD, Rhee I, Mauro NA, Pan D, Hu G, Scott MJ, Fuhrhop RW, Gaffiney PJ, Wickline SA, Lanza GM: Conquering the dark side colloidal iron oxide nanoparticles. ACS NANO 2009, 3: 3917–3926. 10.1021/nn900819y
Hong S, Rhee I: Signal loss in the T2-weighted magnetic resonance images by using an USPIO-particle contrast agent. J Korean Phys Soc 2007, 51: 1453–1456. 10.3938/jkps.51.1453
Ahmad T, Rhee I, Hong S, Chang Y, Lee J: Ni-Fe2O4nanoparticles as contrast agents for magnetic resonance imaging. J Nanosci Nanotech 2011, 11: 5645–5650. 10.1166/jnn.2011.4502
Zhang S, Niu H, Hu Z, Cai Y, Shi Y: Preparation of carbon-coated Fe3O4nanoparticles and their application for solid-phase extraction of polycyclic aromatic hydrocarbons from environmental water samples. J Chromatogr A 2010, 1217: 4757–4764. 10.1016/j.chroma.2010.05.035
Wang Z, Guo H, Yu Y, He N: Synthesis and characterization of a novel magnetic carrier with its composition of Fe3O4/carbon using hydrothermal reaction. J Magn Magn Mater 2006, 302: 397–404. 10.1016/j.jmmm.2005.09.044
Okuhata Y: Delivery of diagnostic agents for magnetic resonance imaging. Adv Drug Delivery Rev 1999, 37: 121–137. 10.1016/S0169-409X(98)00103-3
This work was supported by the National Research Foundation of Korea (2010-0021315) and was also supported by the Basic Science Research Program through the National Research Foundation of Korea(NRF) grant funded by the Korean government (MEST; 2009-0072413) and the Nuclear R&D Program (grant code: 20090081817) of the NRF funded by MEST.
The authors declare that they have no competing interests.
HB and TA synthesized the carbon-coated nanoparticles. SH carried out FTIR and DLS measurements. YC and SJ performed MRI measurements to determine T1 and T2 relaxivities. IR designed the experiments and wrote the manuscript with TA. All authors read and approved the final manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 2.0 International License ( https://creativecommons.org/licenses/by/2.0 ), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
About this article
Cite this article
Bae, H., Ahmad, T., Rhee, I. et al. Carbon-coated iron oxide nanoparticles as contrast agents in magnetic resonance imaging. Nanoscale Res Lett 7, 44 (2012). https://doi.org/10.1186/1556-276X-7-44
- iron oxide nanoparticles
- carbon-coated nanoparticles